Mechanical and Durability Performance of Polyacrylonitrile ... fiber reinforced concrete and the...
Embed Size (px)
Transcript of Mechanical and Durability Performance of Polyacrylonitrile ... fiber reinforced concrete and the...
DOI: http://dx.doi.org/10.1590/1516-1439.021915 Materials Research. 2015; 18(6): 1298-1303 © 2015
1. Introduction As for its low cost and satisfactory engineering properties,
concrete is widely applied in the infrastructure construction in the world1-3. However, concrete is typically characterized as quasi-brittle and low tensile strength. When the concrete is loaded, the initially and discontinuous microcracks are appeared in this matrix, which limits the development of concrete science. The added micro-fiber can overcome these weaknesses and control the crack propagation effectively, which finally improved the mechanical and durability performance of concrete.
PAN fiber, shortened for Polyacrylonitrile Fiber, was a kind of synthetic fiber which made by acylonitrile copolymer. Recently, experimental tests have shown PAN fiber to have an average strength of 40 cN/dtex. Their high stiffness, tensile strength, chemical resistance, and electrical and thermal conductivity make them attractive for applying as reinforcement for specimens, including concrete materials. In the lastest decade, as a kind of green material for concrete, PAN fiber is considered as a promising candidate in a wide range of applications4-8. Xu et al.9 studied the performance of fiber reinforced asphalt concrete (AC) under environmental temperature and water effects and he found that the fibers have significantly improved AC’s rutting resistance, fatigue life, and toughness. The flexural strength and ultimate flexural strain, and the split indirect tensile strength (SITS) at low temperature have also improved. Yao & Feng10 researched the durability of freezing/thawing resistance of polyacrylonitrile fiber reinforced concrete and the results indicated that the polyacrylonitrile fibers were of firm interface combined with concrete. The fibers have meshwork adjective function of resisting fatigue destruction. By adding suitable volume
fraction of fibers, the durability of freezing/thawing resistance of concrete will be improved remarkably. Sun et al.11 put the short polyacrylonitrile-based carbon fibers (0.2~2.0 wt.%) in concrete and tested the thermoelectric power (TEP) and conductivity. TEP in CFRC increases, with the content of short carbon fiber increasing from 0.2 to 1.0 wt.%. As the content of carbon fiber reaches 1.2 wt.%, TEP decreases abruptly. In the end, TEP is almost maintained marginally with increasing content of carbon fiber from 1.4 to 2.0 wt.%.
In this paper, the impact toughness, autogenous shrinkage, chloride penetration resistance, permeability resistance and abrasion resistance performance of prepared concrete reinforced with PAN fiber were researched. The PAN fiber volume concentration percentages of cement were 0, 0.5%, 1.0%, 1.5% and 2.0% by cement, respectively. Finally, MIP was used to characterize the pore parameters of PAN fiber reinforced concrete specimens.
2. Experimental 2.1. Materials
The used materials for concrete were Ordinary Portland cement (42.5R), natural river sand (fineness modulus of 2.9) and natural coarse aggregate (maximum particle size of 25 mm, 5~15mm is 30% and 15~25 mm is 70%). Ordinary Portland cement (42.5R) was provided by Anhui Conch Cement Co., Ltd., and the correspondingly parameters were shown in Table 1. Natural river sand and natural coarse aggregate were both provided by Xi’an Jingtian Building Materials Co., Ltd. Polycarboxylate superplasticizer (PS), with water reduction efficiency of 30%, was purchased from Xi’an Shenghua New Building Materials Co., Ltd. PAN fiber
Mechanical and Durability Performance of Polyacrylonitrile Fiber Reinforced Concrete
aSchool of Civil Engineering, Xi’an University of Architecture and Technology, Xi’an 710000, China
Received: August 12, 2015; Revised: October 5, 2015
In this paper, the impact toughness, autogenous shrinkage, chloride penetration resistance, permeability resistance and abrasion resistance performance of prepared concrete reinforced with Polyacrylonitrile fiber (PAN fiber) were researched. The PAN fiber volume concentration percentages of cement were 0, 0.5%, 1.0%, 1.5% and 2.0%, respectively. The results showed that with the addition of PAN fiber, the toughness and durability performance were improved. Compared to the reference sample, the impact energy was significantly improved. The absorbed energy prevent specimens from deterioration by the mechanisms of matrix cracking, PAN fiber/matrix interface debonding, fiber pull-out and fiber rupture. Meanwhile, the autogenous shrinkage, chloride penetration resistance, permeability resistance and abrasion resistance performance were improved. Mercury intrusion porosimetry (MIP) technique found that concrete with PAN fiber has a better pore characterization. Among these specimens, the maximum improvement was obtained with 1.0 vol.% PAN fiber.
Keywords: concrete, polyacrylonitrile fiber (PAN fiber), impact energy, toughness, autogenous shrinkage, chloride penetration resistance, permeability resistance, abrasion resistance
Mechanical and Durability Performance of Polyacrylonitrile Fiber Reinforced Concrete2015; 18(6) 1299
was supplied from Shandong Binzhou Qisu Materials Co., Ltd. and the physical parameters were shown in Table 2.
2.2. Sample preparation The detailed mix proportion of prepared PAN fiber
reinforced concrete was shown in Table 3. The water to cement ratio was 0.38 and the sand to aggregate ratio was 40%, respectively. The preparation procedures involved: (1) cement, natural river sand and natural coarse aggregate were poured into the laboratory concrete mixer and for 2 minutes’ mixing; (2) adding PAN fiber for another 1 minutes’ mixing; (3) adding the weighed water (including 0.8% PS) in 30 seconds; (4) the final mixing was applied in 2 minute; (5) casting the prepared PAN fiber reinforced paste into the shaped molds and a electric vibrator was used to ensure good compaction. All specimens were demolded after 1 day and cured in a standard environment condition in moist room with a temperature of 20±1 °C and relative humidity of not less than 95%.
2.3. Testing procedures During the impact toughness test, a steel ball (4.5 kg),
with no initial velocity, was dropped repeatly on the prepared PAN fiber reinforced concrete specimens of 457 mm height. The number of blows of first crack initiation and ultimate failure were recorded. The correspondingly equations were shown as follows:
H= gt (1)
Impact energy during each drop,
U= mV (3)
The autogenous shrinkage of PAN fiber reinforced concrete specimens was performed by specimens (100 mm×100mm×400 mm). The stainless steel gage studs were glued directly to the surface of the specimens maintaining a certain length. A length comparator was used to measure the distance during this procedure. From these measurements, the autogenous shrinkage was calculated.
Chloride penetration resistance performance of PAN fiber reinforced concrete specimens was performed on the cylindrical specimens with 50 mm height and 100 mm diameter. Firstly, the prepared PAN fiber reinforced concrete specimens were carried out for a saturation process for 24 hours, then fixed in the shaped molds. During this test, the 3.0% sodium chloride solution and 0.3 mol/L sodium hydroxide solution were used. After 6 hours’ circular telegram process, the electric flux of PAN fiber reinforced concrete specimens was recorded. Permeability resistance performance of PAN fiber reinforced concrete specimens were tested by using cylindrical specimens (50 mm height and 100 mm diameter). One surface was exposed on water and they were weighed after 1, 5, 10, 20, and 30 minutes, 1, 2, 3, 4, 5 and 6 hours, and 1, 2, 3, 4, 5, 6, 7, 8 and 9 days12. A concrete abrasion device was used in abrasion resistance test with a speed of 200 r/min and exerting load force of 100 N. Three 2-minute abrasion periods were repeated on the surface of each PAN fiber reinforced concrete specimens and the abrasion weight loss was weighed. Each test was performed on three replicated specimens.
An automated mercury porosimeter (AUTOPORE IV 9500 series, Micromertics Instrument Corp., USA), with two low-pressure stations plus one high-pressure station and a maximum pressure of 33,000 psia for measurements, was used to measure the correspondingly porosity and the pore size distribution. During this procedure, PAN fiber reinforced concrete specimens were soaked in ethanol for about 1 day to stop the cement hydration reaction, and then dried in an oven at 60 °C.
Table 1. The detailed physical parameters of Ordinary Portland cement 42.5R.
Specific surface area
Loss on ignition (%)
Setting time (min)
Flexural strength (MPa)
Compressive strength (MPa)
Initial setting Final setting 3d 28d 3d 28d
321 2.68 195 260 5.6 9.1 31.7 59.2
Table 2. The detailed physical parameters of PAN fiber.
PAN fiber Llength(mm) Diameter
Tensile strength (MPa)
Elastic modulus (MPa)
— 10 20~40 ≥500 ≥3850 10~28 0.91 High
Table 3. Mix proportion of the prepared PAN fiber reinforced concrete.
No. Water to cement ratio Cement(kg) Coarse aggregate
(kg) River sand
(kg) Water (kg) PS (%)
PAN fibers (vol.%)
PAN-0 0.38 500 900 600 190 0.8 0 PAN-1 0.38 500 900 600 190 0.8 0.5 PAN-2 0.38 500 900 600 190 0.8 1.0 PAN-3 0.38 500 90